#------------------------------------------------------------------------------
#$Date: 2016-03-23 21:05:52 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179439 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/36/4333600.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4333600
loop_
_publ_author_name
'M. Falmbigl'
'F. Kneidinger'
'M. Chen'
'A. Grytsiv'
'H. Michor'
'E. Royanian'
'E. Bauer'
'H. Effenberger'
'R. Podloucky'
'P. Rogl'
_publ_section_title
;
 Cage-Forming Compounds in the Ba-Rh-Ge System: From Thermoelectrics to
 Superconductivity
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              931
_journal_page_last               943
_journal_paper_doi               10.1021/ic302139r
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Ba8 Ge45 Rh'
_chemical_formula_weight         4468.18
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           223
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   10.708(2)
_cell_length_b                   10.708(2)
_cell_length_c                   10.708(2)
_cell_measurement_temperature    573(2)
_cell_volume                     1227.8(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      573(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0472
_diffrn_reflns_av_sigmaI/netI    0.0336
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            1652
_diffrn_reflns_theta_full        34.95
_diffrn_reflns_theta_max         34.95
_diffrn_reflns_theta_min         2.69
_exptl_absorpt_coefficient_mu    33.660
_exptl_absorpt_correction_T_max  0.4317
_exptl_absorpt_correction_T_min  0.2839
_exptl_crystal_density_diffrn    6.043
_exptl_crystal_F_000             1933
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.148
_refine_diff_density_min         -0.846
_refine_diff_density_rms         0.182
_refine_ls_extinction_coef       0.00023(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.170
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     24
_refine_ls_number_reflns         516
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.170
_refine_ls_R_factor_all          0.0654
_refine_ls_R_factor_gt           0.0279
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+6.9168P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0402
_refine_ls_wR_factor_ref         0.0447
_reflns_number_gt                341
_reflns_number_total             516
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302139r_si_002_3.cif
_cod_data_source_block           k1_300K
_cod_database_code               4333600
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'x+1/2, z+1/2, -y+1/2'
'-x+1/2, z+1/2, y+1/2'
'-x+1/2, -z+1/2, -y+1/2'
'x+1/2, -z+1/2, y+1/2'
'z+1/2, y+1/2, -x+1/2'
'z+1/2, -y+1/2, x+1/2'
'-z+1/2, y+1/2, x+1/2'
'-z+1/2, -y+1/2, -x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y-1/2, -x-1/2, z-1/2'
'y-1/2, x-1/2, z-1/2'
'-y-1/2, x-1/2, -z-1/2'
'y-1/2, -x-1/2, -z-1/2'
'-x-1/2, -z-1/2, y-1/2'
'x-1/2, -z-1/2, -y-1/2'
'x-1/2, z-1/2, y-1/2'
'-x-1/2, z-1/2, -y-1/2'
'-z-1/2, -y-1/2, x-1/2'
'-z-1/2, y-1/2, -x-1/2'
'z-1/2, -y-1/2, -x-1/2'
'z-1/2, y-1/2, x-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.0000 0.0000 0.0000 0.0151(2) Uani 1 24 d S
Ba2 Ba 0.2500 0.0000 0.5000 0.0422(3) Uani 1 8 d S
Rh1 Rh 0.2500 0.5000 0.0000 0.0151(6) Uani 0.20 8 d SP
Ge2 Ge 0.2500 0.5000 0.0000 0.0151(6) Uani 0.457(6) 8 d SP
Ge1 Ge 0.18364(4) 0.18364(4) 0.18364(4) 0.01769(18) Uani 1 3 d S
Ge3 Ge 0.0000 0.1156(12) 0.3092(12) 0.0174(10) Uani 0.64(7) 2 d SP
Ge4 Ge 0.0000 0.1334(19) 0.335(3) 0.0223(18) Uani 0.36(7) 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rh Rh -1.1178 0.9187 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ge1 Ba1 Ge1 180.00(2) 25 .
Ge1 Ba1 Ge1 109.5 25 28
Ge1 Ba1 Ge1 70.5 . 28
Ge1 Ba1 Ge1 70.5 25 4
Ge1 Ba1 Ge1 109.5 . 4
Ge1 Ba1 Ge1 180.00(2) 28 4
Ge1 Ba1 Ge1 109.5 25 27
Ge1 Ba1 Ge1 70.5 . 27
Ge1 Ba1 Ge1 109.5 28 27
Ge1 Ba1 Ge1 70.5 4 27
Ge1 Ba1 Ge1 70.5 25 3
Ge1 Ba1 Ge1 109.5 . 3
Ge1 Ba1 Ge1 70.5 28 3
Ge1 Ba1 Ge1 109.5 4 3
Ge1 Ba1 Ge1 180.00(3) 27 3
Ge1 Ba1 Ge1 109.5 25 26
Ge1 Ba1 Ge1 70.5 . 26
Ge1 Ba1 Ge1 109.5 28 26
Ge1 Ba1 Ge1 70.5 4 26
Ge1 Ba1 Ge1 109.5 27 26
Ge1 Ba1 Ge1 70.5 3 26
Ge1 Ba1 Ge1 70.5 25 2
Ge1 Ba1 Ge1 109.5 . 2
Ge1 Ba1 Ge1 70.5 28 2
Ge1 Ba1 Ge1 109.5 4 2
Ge1 Ba1 Ge1 70.5 27 2
Ge1 Ba1 Ge1 109.5 3 2
Ge1 Ba1 Ge1 180.00(3) 26 2
Ge1 Ba1 Ge3 42.01(8) 25 33
Ge1 Ba1 Ge3 137.99(8) . 33
Ge1 Ba1 Ge3 109.79(12) 28 33
Ge1 Ba1 Ge3 70.21(12) 4 33
Ge1 Ba1 Ge3 70.21(12) 27 33
Ge1 Ba1 Ge3 109.79(12) 3 33
Ge1 Ba1 Ge3 137.99(8) 26 33
Ge1 Ba1 Ge3 42.01(8) 2 33
Ge1 Ba1 Ge3 137.99(8) 25 9
Ge1 Ba1 Ge3 42.01(8) . 9
Ge1 Ba1 Ge3 70.21(12) 28 9
Ge1 Ba1 Ge3 109.79(12) 4 9
Ge1 Ba1 Ge3 109.79(12) 27 9
Ge1 Ba1 Ge3 70.21(12) 3 9
Ge1 Ba1 Ge3 42.01(8) 26 9
Ge1 Ba1 Ge3 137.99(8) 2 9
Ge3 Ba1 Ge3 180.00(15) 33 9
Ge1 Ba1 Ge3 42.01(8) 25 29
Ge1 Ba1 Ge3 137.99(8) . 29
Ge1 Ba1 Ge3 70.21(12) 28 29
Ge1 Ba1 Ge3 109.79(12) 4 29
Ge1 Ba1 Ge3 137.99(8) 27 29
Ge1 Ba1 Ge3 42.01(8) 3 29
Ge1 Ba1 Ge3 109.79(12) 26 29
Ge1 Ba1 Ge3 70.21(12) 2 29
Ge3 Ba1 Ge3 70.85(12) 33 29
Ge3 Ba1 Ge3 109.15(12) 9 29
Ge1 Ba1 Ge3 137.99(8) 25 5
Ge1 Ba1 Ge3 42.01(8) . 5
Ge1 Ba1 Ge3 109.79(12) 28 5
Ge1 Ba1 Ge3 70.21(12) 4 5
Ge1 Ba1 Ge3 42.01(8) 27 5
Ge1 Ba1 Ge3 137.99(8) 3 5
Ge1 Ba1 Ge3 70.21(12) 26 5
Ge1 Ba1 Ge3 109.79(12) 2 5
Ge3 Ba1 Ge3 109.15(12) 33 5
Ge3 Ba1 Ge3 70.85(12) 9 5
Ge3 Ba1 Ge3 180.0(5) 29 5
Ge4 Ba2 Ge4 172.1(11) 41_666 2
Ge4 Ba2 Ge4 48.0(8) 41_666 42_666
Ge4 Ba2 Ge4 125.5(3) 2 42_666
Ge4 Ba2 Ge4 125.5(3) 41_666 .
Ge4 Ba2 Ge4 48.0(8) 2 .
Ge4 Ba2 Ge4 99.8(4) 42_666 .
Ge4 Ba2 Ge4 60.5(10) 41_666 18_545
Ge4 Ba2 Ge4 125.5(3) 2 18_545
Ge4 Ba2 Ge4 80.7(5) 42_666 18_545
Ge4 Ba2 Ge4 172.1(11) . 18_545
Ge4 Ba2 Ge4 125.5(3) 41_666 25_556
Ge4 Ba2 Ge4 60.5(10) 2 25_556
Ge4 Ba2 Ge4 172.1(11) 42_666 25_556
Ge4 Ba2 Ge4 80.7(5) . 25_556
Ge4 Ba2 Ge4 99.8(4) 18_545 25_556
Ge4 Ba2 Ge4 80.7(5) 41_666 17_545
Ge4 Ba2 Ge4 99.8(4) 2 17_545
Ge4 Ba2 Ge4 60.5(10) 42_666 17_545
Ge4 Ba2 Ge4 125.5(3) . 17_545
Ge4 Ba2 Ge4 48.0(8) 18_545 17_545
Ge4 Ba2 Ge4 125.5(3) 25_556 17_545
Ge4 Ba2 Ge4 99.8(4) 41_666 26_556
Ge4 Ba2 Ge4 80.7(5) 2 26_556
Ge4 Ba2 Ge4 125.5(3) 42_666 26_556
Ge4 Ba2 Ge4 60.5(10) . 26_556
Ge4 Ba2 Ge4 125.5(3) 18_545 26_556
Ge4 Ba2 Ge4 48.0(8) 25_556 26_556
Ge4 Ba2 Ge4 172.1(11) 17_545 26_556
Ge4 Ba2 Ge3 5.2(3) 41_666 41_666
Ge4 Ba2 Ge3 166.9(8) 2 41_666
Ge4 Ba2 Ge3 44.3(6) 42_666 41_666
Ge4 Ba2 Ge3 120.72(19) . 41_666
Ge4 Ba2 Ge3 65.1(7) 18_545 41_666
Ge4 Ba2 Ge3 128.8(4) 25_556 41_666
Ge4 Ba2 Ge3 81.9(3) 17_545 41_666
Ge4 Ba2 Ge3 99.38(10) 26_556 41_666
Ge4 Ba2 Ge3 166.9(8) 41_666 2
Ge4 Ba2 Ge3 5.2(3) 2 2
Ge4 Ba2 Ge3 120.72(19) 42_666 2
Ge4 Ba2 Ge3 44.3(6) . 2
Ge4 Ba2 Ge3 128.8(4) 18_545 2
Ge4 Ba2 Ge3 65.1(7) 25_556 2
Ge4 Ba2 Ge3 99.38(10) 17_545 2
Ge4 Ba2 Ge3 81.9(3) 26_556 2
Ge3 Ba2 Ge3 161.7(5) 41_666 2
Ge4 Ba2 Ge3 128.8(4) 41_666 .
Ge4 Ba2 Ge3 44.3(6) 2 .
Ge4 Ba2 Ge3 99.38(10) 42_666 .
Ge4 Ba2 Ge3 5.2(3) . .
Ge4 Ba2 Ge3 166.9(8) 18_545 .
Ge4 Ba2 Ge3 81.9(3) 25_556 .
Ge4 Ba2 Ge3 120.72(19) 17_545 .
Ge4 Ba2 Ge3 65.1(7) 26_556 .
Ge3 Ba2 Ge3 123.83(12) 41_666 .
Ge3 Ba2 Ge3 40.4(4) 2 .
Ge4 Ba2 Ge3 44.3(6) 41_666 42_666
Ge4 Ba2 Ge3 128.8(4) 2 42_666
Ge4 Ba2 Ge3 5.2(3) 42_666 42_666
Ge4 Ba2 Ge3 99.38(10) . 42_666
Ge4 Ba2 Ge3 81.9(3) 18_545 42_666
Ge4 Ba2 Ge3 166.9(8) 25_556 42_666
Ge4 Ba2 Ge3 65.1(7) 17_545 42_666
Ge4 Ba2 Ge3 120.72(19) 26_556 42_666
Ge3 Ba2 Ge3 40.4(4) 41_666 42_666
Ge3 Ba2 Ge3 123.83(12) 2 42_666
Ge3 Ba2 Ge3 99.42(19) . 42_666
Ge4 Ba2 Ge3 65.1(7) 41_666 18_545
Ge4 Ba2 Ge3 120.72(19) 2 18_545
Ge4 Ba2 Ge3 81.9(3) 42_666 18_545
Ge4 Ba2 Ge3 166.9(8) . 18_545
Ge4 Ba2 Ge3 5.2(3) 18_545 18_545
Ge4 Ba2 Ge3 99.38(10) 25_556 18_545
Ge4 Ba2 Ge3 44.3(6) 17_545 18_545
Ge4 Ba2 Ge3 128.8(4) 26_556 18_545
Ge3 Ba2 Ge3 69.4(4) 41_666 18_545
Ge3 Ba2 Ge3 123.83(12) 2 18_545
Ge3 Ba2 Ge3 161.7(5) . 18_545
Ge3 Ba2 Ge3 83.5(2) 42_666 18_545
Ge4 Ba2 Ge3 120.72(19) 41_666 25_556
Ge4 Ba2 Ge3 65.1(7) 2 25_556
Ge4 Ba2 Ge3 166.9(8) 42_666 25_556
Ge4 Ba2 Ge3 81.9(3) . 25_556
Ge4 Ba2 Ge3 99.38(10) 18_545 25_556
Ge4 Ba2 Ge3 5.2(3) 25_556 25_556
Ge4 Ba2 Ge3 128.8(4) 17_545 25_556
Ge4 Ba2 Ge3 44.3(6) 26_556 25_556
Ge3 Ba2 Ge3 123.83(12) 41_666 25_556
Ge3 Ba2 Ge3 69.4(4) 2 25_556
Ge3 Ba2 Ge3 83.5(2) . 25_556
Ge3 Ba2 Ge3 161.7(5) 42_666 25_556
Ge3 Ba2 Ge3 99.42(19) 18_545 25_556
Ge4 Ba2 Ge3 81.9(3) 41_666 17_545
Ge4 Ba2 Ge3 99.38(10) 2 17_545
Ge4 Ba2 Ge3 65.1(7) 42_666 17_545
Ge4 Ba2 Ge3 128.8(4) . 17_545
Ge4 Ba2 Ge3 44.3(6) 18_545 17_545
Ge4 Ba2 Ge3 120.72(19) 25_556 17_545
Ge4 Ba2 Ge3 5.2(3) 17_545 17_545
Ge4 Ba2 Ge3 166.9(8) 26_556 17_545
Ge3 Ba2 Ge3 83.5(2) 41_666 17_545
Ge3 Ba2 Ge3 99.42(19) 2 17_545
Ge3 Ba2 Ge3 123.83(12) . 17_545
Ge3 Ba2 Ge3 69.4(4) 42_666 17_545
Ge3 Ba2 Ge3 40.4(4) 18_545 17_545
Ge3 Ba2 Ge3 123.83(12) 25_556 17_545
Ge4 Ba2 Ge3 99.38(10) 41_666 26_556
Ge4 Ba2 Ge3 81.9(3) 2 26_556
Ge4 Ba2 Ge3 128.8(4) 42_666 26_556
Ge4 Ba2 Ge3 65.1(7) . 26_556
Ge4 Ba2 Ge3 120.72(19) 18_545 26_556
Ge4 Ba2 Ge3 44.3(6) 25_556 26_556
Ge4 Ba2 Ge3 166.9(8) 17_545 26_556
Ge4 Ba2 Ge3 5.2(3) 26_556 26_556
Ge3 Ba2 Ge3 99.42(19) 41_666 26_556
Ge3 Ba2 Ge3 83.5(2) 2 26_556
Ge3 Ba2 Ge3 69.4(4) . 26_556
Ge3 Ba2 Ge3 123.83(12) 42_666 26_556
Ge3 Ba2 Ge3 123.83(12) 18_545 26_556
Ge3 Ba2 Ge3 40.4(4) 25_556 26_556
Ge3 Ba2 Ge3 161.7(5) 17_545 26_556
Ge4 Ba2 Ge2 34.3(6) 41_666 33_656
Ge4 Ba2 Ge2 153.5(5) 2 33_656
Ge4 Ba2 Ge2 75.4(2) 42_666 33_656
Ge4 Ba2 Ge2 153.5(5) . 33_656
Ge4 Ba2 Ge2 34.3(6) 18_545 33_656
Ge4 Ba2 Ge2 100.5(4) 25_556 33_656
Ge4 Ba2 Ge2 75.4(2) 17_545 33_656
Ge4 Ba2 Ge2 100.5(4) 26_556 33_656
Ge3 Ba2 Ge2 39.5(3) 41_666 33_656
Ge3 Ba2 Ge2 158.5(3) 2 33_656
Ge3 Ba2 Ge2 158.5(3) . 33_656
Ge3 Ba2 Ge2 73.53(15) 42_666 33_656
Ge3 Ba2 Ge2 39.5(3) 18_545 33_656
Ge3 Ba2 Ge2 97.18(16) 25_556 33_656
Ge3 Ba2 Ge2 73.53(15) 17_545 33_656
Ge3 Ba2 Ge2 97.18(16) 26_556 33_656
Ge4 Ba2 Ge2 153.5(5) 41_666 29_556
Ge4 Ba2 Ge2 34.3(6) 2 29_556
Ge4 Ba2 Ge2 153.5(5) 42_666 29_556
Ge4 Ba2 Ge2 75.4(2) . 29_556
Ge4 Ba2 Ge2 100.5(4) 18_545 29_556
Ge4 Ba2 Ge2 34.3(6) 25_556 29_556
Ge4 Ba2 Ge2 100.5(4) 17_545 29_556
Ge4 Ba2 Ge2 75.4(2) 26_556 29_556
Ge3 Ba2 Ge2 158.5(3) 41_666 29_556
Ge3 Ba2 Ge2 39.5(3) 2 29_556
Ge3 Ba2 Ge2 73.53(15) . 29_556
Ge3 Ba2 Ge2 158.5(3) 42_666 29_556
Ge3 Ba2 Ge2 97.18(16) 18_545 29_556
Ge3 Ba2 Ge2 39.5(3) 25_556 29_556
Ge3 Ba2 Ge2 97.18(16) 17_545 29_556
Ge3 Ba2 Ge2 73.53(15) 26_556 29_556
Ge2 Ba2 Ge2 120.0 33_656 29_556
Ge4 Ba2 Rh1 34.3(6) 41_666 33_656
Ge4 Ba2 Rh1 153.5(5) 2 33_656
Ge4 Ba2 Rh1 75.4(2) 42_666 33_656
Ge4 Ba2 Rh1 153.5(5) . 33_656
Ge4 Ba2 Rh1 34.3(6) 18_545 33_656
Ge4 Ba2 Rh1 100.5(4) 25_556 33_656
Ge4 Ba2 Rh1 75.4(2) 17_545 33_656
Ge4 Ba2 Rh1 100.5(4) 26_556 33_656
Ge3 Ba2 Rh1 39.5(3) 41_666 33_656
Ge3 Ba2 Rh1 158.5(3) 2 33_656
Ge3 Ba2 Rh1 158.5(3) . 33_656
Ge3 Ba2 Rh1 73.53(15) 42_666 33_656
Ge3 Ba2 Rh1 39.5(3) 18_545 33_656
Ge3 Ba2 Rh1 97.18(16) 25_556 33_656
Ge3 Ba2 Rh1 73.53(15) 17_545 33_656
Ge3 Ba2 Rh1 97.18(16) 26_556 33_656
Ge2 Ba2 Rh1 0.0 33_656 33_656
Ge2 Ba2 Rh1 120.0 29_556 33_656
Ge4 Ba2 Rh1 153.5(5) 41_666 29_556
Ge4 Ba2 Rh1 34.3(6) 2 29_556
Ge4 Ba2 Rh1 153.5(5) 42_666 29_556
Ge4 Ba2 Rh1 75.4(2) . 29_556
Ge4 Ba2 Rh1 100.5(4) 18_545 29_556
Ge4 Ba2 Rh1 34.3(6) 25_556 29_556
Ge4 Ba2 Rh1 100.5(4) 17_545 29_556
Ge4 Ba2 Rh1 75.4(2) 26_556 29_556
Ge3 Ba2 Rh1 158.5(3) 41_666 29_556
Ge3 Ba2 Rh1 39.5(3) 2 29_556
Ge3 Ba2 Rh1 73.53(15) . 29_556
Ge3 Ba2 Rh1 158.5(3) 42_666 29_556
Ge3 Ba2 Rh1 97.18(16) 18_545 29_556
Ge3 Ba2 Rh1 39.5(3) 25_556 29_556
Ge3 Ba2 Rh1 97.18(16) 17_545 29_556
Ge3 Ba2 Rh1 73.53(15) 26_556 29_556
Ge2 Ba2 Rh1 120.0 33_656 29_556
Ge2 Ba2 Rh1 0.0 29_556 29_556
Rh1 Ba2 Rh1 120.0 33_656 29_556
Ge4 Ba2 Ge2 75.4(2) 41_666 9
Ge4 Ba2 Ge2 100.5(4) 2 9
Ge4 Ba2 Ge2 34.3(6) 42_666 9
Ge4 Ba2 Ge2 100.5(4) . 9
Ge4 Ba2 Ge2 75.4(2) 18_545 9
Ge4 Ba2 Ge2 153.5(5) 25_556 9
Ge4 Ba2 Ge2 34.3(6) 17_545 9
Ge4 Ba2 Ge2 153.5(5) 26_556 9
Ge3 Ba2 Ge2 73.53(15) 41_666 9
Ge3 Ba2 Ge2 97.18(16) 2 9
Ge3 Ba2 Ge2 97.18(16) . 9
Ge3 Ba2 Ge2 39.5(3) 42_666 9
Ge3 Ba2 Ge2 73.53(15) 18_545 9
Ge3 Ba2 Ge2 158.5(3) 25_556 9
Ge3 Ba2 Ge2 39.5(3) 17_545 9
Ge3 Ba2 Ge2 158.5(3) 26_556 9
Ge2 Ba2 Ge2 90.0 33_656 9
Ge2 Ba2 Ge2 120.0 29_556 9
Rh1 Ba2 Ge2 90.0 33_656 9
Rh1 Ba2 Ge2 120.0 29_556 9
Ge4 Ba2 Rh1 75.4(2) 41_666 9
Ge4 Ba2 Rh1 100.5(4) 2 9
Ge4 Ba2 Rh1 34.3(6) 42_666 9
Ge4 Ba2 Rh1 100.5(4) . 9
Ge4 Ba2 Rh1 75.4(2) 18_545 9
Ge4 Ba2 Rh1 153.5(5) 25_556 9
Ge4 Ba2 Rh1 34.3(6) 17_545 9
Ge4 Ba2 Rh1 153.5(5) 26_556 9
Ge3 Ba2 Rh1 73.53(15) 41_666 9
Ge3 Ba2 Rh1 97.18(16) 2 9
Ge3 Ba2 Rh1 97.18(16) . 9
Ge3 Ba2 Rh1 39.5(3) 42_666 9
Ge3 Ba2 Rh1 73.53(15) 18_545 9
Ge3 Ba2 Rh1 158.5(3) 25_556 9
Ge3 Ba2 Rh1 39.5(3) 17_545 9
Ge3 Ba2 Rh1 158.5(3) 26_556 9
Ge2 Ba2 Rh1 90.0 33_656 9
Ge2 Ba2 Rh1 120.0 29_556 9
Rh1 Ba2 Rh1 90.0 33_656 9
Rh1 Ba2 Rh1 120.0 29_556 9
Ge2 Ba2 Rh1 0.0 9 9
Ge4 Ba2 Ge2 100.5(4) 41_666 5
Ge4 Ba2 Ge2 75.4(2) 2 5
Ge4 Ba2 Ge2 100.5(4) 42_666 5
Ge4 Ba2 Ge2 34.3(6) . 5
Ge4 Ba2 Ge2 153.5(5) 18_545 5
Ge4 Ba2 Ge2 75.4(2) 25_556 5
Ge4 Ba2 Ge2 153.5(5) 17_545 5
Ge4 Ba2 Ge2 34.3(6) 26_556 5
Ge3 Ba2 Ge2 97.18(16) 41_666 5
Ge3 Ba2 Ge2 73.53(15) 2 5
Ge3 Ba2 Ge2 39.5(3) . 5
Ge3 Ba2 Ge2 97.18(16) 42_666 5
Ge3 Ba2 Ge2 158.5(3) 18_545 5
Ge3 Ba2 Ge2 73.53(15) 25_556 5
Ge3 Ba2 Ge2 158.5(3) 17_545 5
Ge3 Ba2 Ge2 39.5(3) 26_556 5
Ge2 Ba2 Ge2 120.0 33_656 5
Ge2 Ba2 Ge2 90.0 29_556 5
Rh1 Ba2 Ge2 120.0 33_656 5
Rh1 Ba2 Ge2 90.0 29_556 5
Ge2 Ba2 Ge2 120.0 9 5
Rh1 Ba2 Ge2 120.0 9 5
Ge4 Ba2 Rh1 100.5(4) 41_666 5
Ge4 Ba2 Rh1 75.4(2) 2 5
Ge4 Ba2 Rh1 100.5(4) 42_666 5
Ge4 Ba2 Rh1 34.3(6) . 5
Ge4 Ba2 Rh1 153.5(5) 18_545 5
Ge4 Ba2 Rh1 75.4(2) 25_556 5
Ge4 Ba2 Rh1 153.5(5) 17_545 5
Ge4 Ba2 Rh1 34.3(6) 26_556 5
Ge3 Ba2 Rh1 97.18(16) 41_666 5
Ge3 Ba2 Rh1 73.53(15) 2 5
Ge3 Ba2 Rh1 39.5(3) . 5
Ge3 Ba2 Rh1 97.18(16) 42_666 5
Ge3 Ba2 Rh1 158.5(3) 18_545 5
Ge3 Ba2 Rh1 73.53(15) 25_556 5
Ge3 Ba2 Rh1 158.5(3) 17_545 5
Ge3 Ba2 Rh1 39.5(3) 26_556 5
Ge2 Ba2 Rh1 120.0 33_656 5
Ge2 Ba2 Rh1 90.0 29_556 5
Rh1 Ba2 Rh1 120.0 33_656 5
Rh1 Ba2 Rh1 90.0 29_556 5
Ge2 Ba2 Rh1 120.0 9 5
Rh1 Ba2 Rh1 120.0 9 5
Ge2 Ba2 Rh1 0.0 5 5
Ge4 Ba2 Ge1 40.0(3) 41_666 37_666
Ge4 Ba2 Ge1 137.0(2) 2 37_666
Ge4 Ba2 Ge1 68.6(5) 42_666 37_666
Ge4 Ba2 Ge1 92.2(5) . 37_666
Ge4 Ba2 Ge1 95.3(6) 18_545 37_666
Ge4 Ba2 Ge1 103.5(5) 25_556 37_666
Ge4 Ba2 Ge1 119.6(3) 17_545 37_666
Ge4 Ba2 Ge1 62.68(19) 26_556 37_666
Ge3 Ba2 Ge1 37.98(10) 41_666 37_666
Ge3 Ba2 Ge1 135.08(15) 2 37_666
Ge3 Ba2 Ge1 96.9(2) . 37_666
Ge3 Ba2 Ge1 63.4(3) 42_666 37_666
Ge3 Ba2 Ge1 100.4(2) 18_545 37_666
Ge3 Ba2 Ge1 98.4(3) 25_556 37_666
Ge3 Ba2 Ge1 121.46(10) 17_545 37_666
Ge3 Ba2 Ge1 63.78(12) 26_556 37_666
Ge2 Ba2 Ge1 61.608(2) 33_656 37_666
Ge2 Ba2 Ge1 136.715(9) 29_556 37_666
Rh1 Ba2 Ge1 61.608(2) 33_656 37_666
Rh1 Ba2 Ge1 136.715(9) 29_556 37_666
Ge2 Ba2 Ge1 102.888(9) 9 37_666
Rh1 Ba2 Ge1 102.888(9) 9 37_666
Ge2 Ba2 Ge1 61.608(2) 5 37_666
Rh1 Ba2 Ge1 61.608(2) 5 37_666
Ge4 Ba2 Ge1 137.0(2) 41_666 27
Ge4 Ba2 Ge1 40.0(3) 2 27
Ge4 Ba2 Ge1 92.2(5) 42_666 27
Ge4 Ba2 Ge1 68.6(5) . 27
Ge4 Ba2 Ge1 103.5(5) 18_545 27
Ge4 Ba2 Ge1 95.3(6) 25_556 27
Ge4 Ba2 Ge1 62.68(19) 17_545 27
Ge4 Ba2 Ge1 119.6(3) 26_556 27
Ge3 Ba2 Ge1 135.08(15) 41_666 27
Ge3 Ba2 Ge1 37.98(10) 2 27
Ge3 Ba2 Ge1 63.4(3) . 27
Ge3 Ba2 Ge1 96.9(2) 42_666 27
Ge3 Ba2 Ge1 98.4(3) 18_545 27
Ge3 Ba2 Ge1 100.4(2) 25_556 27
Ge3 Ba2 Ge1 63.78(12) 17_545 27
Ge3 Ba2 Ge1 121.46(10) 26_556 27
Ge2 Ba2 Ge1 136.715(9) 33_656 27
Ge2 Ba2 Ge1 61.608(2) 29_556 27
Rh1 Ba2 Ge1 136.715(9) 33_656 27
Rh1 Ba2 Ge1 61.608(2) 29_556 27
Ge2 Ba2 Ge1 61.608(2) 9 27
Rh1 Ba2 Ge1 61.608(2) 9 27
Ge2 Ba2 Ge1 102.888(9) 5 27
Rh1 Ba2 Ge1 102.888(9) 5 27
Ge1 Ba2 Ge1 150.755(15) 37_666 27
Ge4 Ba2 Ge1 119.6(3) 41_666 39_656
Ge4 Ba2 Ge1 62.68(19) 2 39_656
Ge4 Ba2 Ge1 95.3(6) 42_666 39_656
Ge4 Ba2 Ge1 103.5(5) . 39_656
Ge4 Ba2 Ge1 68.6(5) 18_545 39_656
Ge4 Ba2 Ge1 92.2(5) 25_556 39_656
Ge4 Ba2 Ge1 40.0(3) 17_545 39_656
Ge4 Ba2 Ge1 137.0(2) 26_556 39_656
Ge3 Ba2 Ge1 121.46(10) 41_666 39_656
Ge3 Ba2 Ge1 63.78(12) 2 39_656
Ge3 Ba2 Ge1 98.4(3) . 39_656
Ge3 Ba2 Ge1 100.4(2) 42_666 39_656
Ge3 Ba2 Ge1 63.4(3) 18_545 39_656
Ge3 Ba2 Ge1 96.9(2) 25_556 39_656
Ge3 Ba2 Ge1 37.98(10) 17_545 39_656
Ge3 Ba2 Ge1 135.08(15) 26_556 39_656
Ge2 Ba2 Ge1 102.888(9) 33_656 39_656
Ge2 Ba2 Ge1 61.608(2) 29_556 39_656
Rh1 Ba2 Ge1 102.888(9) 33_656 39_656
Rh1 Ba2 Ge1 61.608(2) 29_556 39_656
Ge2 Ba2 Ge1 61.608(2) 9 39_656
Rh1 Ba2 Ge1 61.608(2) 9 39_656
Ge2 Ba2 Ge1 136.715(9) 5 39_656
Rh1 Ba2 Ge1 136.715(9) 5 39_656
Ge1 Ba2 Ge1 159.434(11) 37_666 39_656
Ge1 Ba2 Ge1 36.021(19) 27 39_656
Ge4 Ba2 Ge1 62.68(19) 41_666 26_556
Ge4 Ba2 Ge1 119.6(3) 2 26_556
Ge4 Ba2 Ge1 103.5(5) 42_666 26_556
Ge4 Ba2 Ge1 95.3(6) . 26_556
Ge4 Ba2 Ge1 92.2(5) 18_545 26_556
Ge4 Ba2 Ge1 68.6(6) 25_556 26_556
Ge4 Ba2 Ge1 137.0(2) 17_545 26_556
Ge4 Ba2 Ge1 40.0(3) 26_556 26_556
Ge3 Ba2 Ge1 63.78(12) 41_666 26_556
Ge3 Ba2 Ge1 121.46(10) 2 26_556
Ge3 Ba2 Ge1 100.4(2) . 26_556
Ge3 Ba2 Ge1 98.4(3) 42_666 26_556
Ge3 Ba2 Ge1 96.9(2) 18_545 26_556
Ge3 Ba2 Ge1 63.4(3) 25_556 26_556
Ge3 Ba2 Ge1 135.08(15) 17_545 26_556
Ge3 Ba2 Ge1 37.98(10) 26_556 26_556
Ge2 Ba2 Ge1 61.608(2) 33_656 26_556
Ge2 Ba2 Ge1 102.888(9) 29_556 26_556
Rh1 Ba2 Ge1 61.608(2) 33_656 26_556
Rh1 Ba2 Ge1 102.888(9) 29_556 26_556
Ge2 Ba2 Ge1 136.715(9) 9 26_556
Rh1 Ba2 Ge1 136.715(9) 9 26_556
Ge2 Ba2 Ge1 61.608(2) 5 26_556
Rh1 Ba2 Ge1 61.608(2) 5 26_556
Ge1 Ba2 Ge1 36.021(19) 37_666 26_556
Ge1 Ba2 Ge1 159.434(11) 27 26_556
Ge1 Ba2 Ge1 150.755(15) 39_656 26_556
Ge4 Ba2 Ge1 103.5(5) 41_666 .
Ge4 Ba2 Ge1 68.6(5) 2 .
Ge4 Ba2 Ge1 62.68(19) 42_666 .
Ge4 Ba2 Ge1 40.0(3) . .
Ge4 Ba2 Ge1 137.0(2) 18_545 .
Ge4 Ba2 Ge1 119.6(3) 25_556 .
Ge4 Ba2 Ge1 92.2(5) 17_545 .
Ge4 Ba2 Ge1 95.3(6) 26_556 .
Ge3 Ba2 Ge1 98.4(3) 41_666 .
Ge3 Ba2 Ge1 63.4(3) 2 .
Ge3 Ba2 Ge1 37.98(10) . .
Ge3 Ba2 Ge1 63.78(12) 42_666 .
Ge3 Ba2 Ge1 135.08(15) 18_545 .
Ge3 Ba2 Ge1 121.46(10) 25_556 .
Ge3 Ba2 Ge1 96.9(2) 17_545 .
Ge3 Ba2 Ge1 100.4(2) 26_556 .
Ge2 Ba2 Ge1 136.715(9) 33_656 .
Ge2 Ba2 Ge1 102.888(9) 29_556 .
Rh1 Ba2 Ge1 136.715(9) 33_656 .
Rh1 Ba2 Ge1 102.888(9) 29_556 .
Ge2 Ba2 Ge1 61.608(2) 9 .
Rh1 Ba2 Ge1 61.608(2) 9 .
Ge2 Ba2 Ge1 61.608(2) 5 .
Rh1 Ba2 Ge1 61.608(2) 5 .
Ge1 Ba2 Ge1 91.826(2) 37_666 .
Ge1 Ba2 Ge1 59.201(17) 27 .
Ge1 Ba2 Ge1 91.826(2) 39_656 .
Ge1 Ba2 Ge1 116.634(12) 26_556 .
Ge4 Ba2 Ge1 68.6(5) 41_666 14
Ge4 Ba2 Ge1 103.5(5) 2 14
Ge4 Ba2 Ge1 40.0(3) 42_666 14
Ge4 Ba2 Ge1 62.68(19) . 14
Ge4 Ba2 Ge1 119.6(3) 18_545 14
Ge4 Ba2 Ge1 137.0(2) 25_556 14
Ge4 Ba2 Ge1 95.3(6) 17_545 14
Ge4 Ba2 Ge1 92.2(5) 26_556 14
Ge3 Ba2 Ge1 63.4(3) 41_666 14
Ge3 Ba2 Ge1 98.4(3) 2 14
Ge3 Ba2 Ge1 63.78(12) . 14
Ge3 Ba2 Ge1 37.98(10) 42_666 14
Ge3 Ba2 Ge1 121.46(10) 18_545 14
Ge3 Ba2 Ge1 135.08(15) 25_556 14
Ge3 Ba2 Ge1 100.4(2) 17_545 14
Ge3 Ba2 Ge1 96.9(2) 26_556 14
Ge2 Ba2 Ge1 102.888(9) 33_656 14
Ge2 Ba2 Ge1 136.715(9) 29_556 14
Rh1 Ba2 Ge1 102.888(9) 33_656 14
Rh1 Ba2 Ge1 136.715(9) 29_556 14
Ge2 Ba2 Ge1 61.608(2) 9 14
Rh1 Ba2 Ge1 61.608(2) 9 14
Ge2 Ba2 Ge1 61.608(2) 5 14
Rh1 Ba2 Ge1 61.608(2) 5 14
Ge1 Ba2 Ge1 59.201(17) 37_666 14
Ge1 Ba2 Ge1 91.826(2) 27 14
Ge1 Ba2 Ge1 116.634(12) 39_656 14
Ge1 Ba2 Ge1 91.826(2) 26_556 14
Ge1 Ba2 Ge1 36.021(19) . 14
Ge4 Ba2 Ge1 95.3(6) 41_666 16_545
Ge4 Ba2 Ge1 92.2(5) 2 16_545
Ge4 Ba2 Ge1 119.6(3) 42_666 16_545
Ge4 Ba2 Ge1 137.0(2) . 16_545
Ge4 Ba2 Ge1 40.0(3) 18_545 16_545
Ge4 Ba2 Ge1 62.68(19) 25_556 16_545
Ge4 Ba2 Ge1 68.6(5) 17_545 16_545
Ge4 Ba2 Ge1 103.5(5) 26_556 16_545
Ge3 Ba2 Ge1 100.4(2) 41_666 16_545
Ge3 Ba2 Ge1 96.9(2) 2 16_545
Ge3 Ba2 Ge1 135.08(15) . 16_545
Ge3 Ba2 Ge1 121.46(10) 42_666 16_545
Ge3 Ba2 Ge1 37.98(10) 18_545 16_545
Ge3 Ba2 Ge1 63.78(12) 25_556 16_545
Ge3 Ba2 Ge1 63.4(3) 17_545 16_545
Ge3 Ba2 Ge1 98.4(3) 26_556 16_545
Ge2 Ba2 Ge1 61.608(2) 33_656 16_545
Ge2 Ba2 Ge1 61.608(2) 29_556 16_545
Rh1 Ba2 Ge1 61.608(2) 33_656 16_545
Rh1 Ba2 Ge1 61.608(2) 29_556 16_545
Ge2 Ba2 Ge1 102.888(9) 9 16_545
Rh1 Ba2 Ge1 102.888(9) 9 16_545
Ge2 Ba2 Ge1 136.715(9) 5 16_545
Rh1 Ba2 Ge1 136.715(9) 5 16_545
Ge1 Ba2 Ge1 116.634(12) 37_666 16_545
Ge1 Ba2 Ge1 91.826(2) 27 16_545
Ge1 Ba2 Ge1 59.201(17) 39_656 16_545
Ge1 Ba2 Ge1 91.826(2) 26_556 16_545
Ge1 Ba2 Ge1 150.755(15) . 16_545
Ge1 Ba2 Ge1 159.434(11) 14 16_545
Ge4 Ba2 Ge1 92.2(5) 41_666 4_556
Ge4 Ba2 Ge1 95.3(6) 2 4_556
Ge4 Ba2 Ge1 137.0(2) 42_666 4_556
Ge4 Ba2 Ge1 119.6(3) . 4_556
Ge4 Ba2 Ge1 62.68(19) 18_545 4_556
Ge4 Ba2 Ge1 40.0(3) 25_556 4_556
Ge4 Ba2 Ge1 103.5(5) 17_545 4_556
Ge4 Ba2 Ge1 68.6(5) 26_556 4_556
Ge3 Ba2 Ge1 96.9(2) 41_666 4_556
Ge3 Ba2 Ge1 100.4(2) 2 4_556
Ge3 Ba2 Ge1 121.46(10) . 4_556
Ge3 Ba2 Ge1 135.08(15) 42_666 4_556
Ge3 Ba2 Ge1 63.78(12) 18_545 4_556
Ge3 Ba2 Ge1 37.98(10) 25_556 4_556
Ge3 Ba2 Ge1 98.4(3) 17_545 4_556
Ge3 Ba2 Ge1 63.4(3) 26_556 4_556
Ge2 Ba2 Ge1 61.608(2) 33_656 4_556
Ge2 Ba2 Ge1 61.608(2) 29_556 4_556
Rh1 Ba2 Ge1 61.608(2) 33_656 4_556
Rh1 Ba2 Ge1 61.608(2) 29_556 4_556
Ge2 Ba2 Ge1 136.715(9) 9 4_556
Rh1 Ba2 Ge1 136.715(9) 9 4_556
Ge2 Ba2 Ge1 102.888(9) 5 4_556
Rh1 Ba2 Ge1 102.888(9) 5 4_556
Ge1 Ba2 Ge1 91.826(2) 37_666 4_556
Ge1 Ba2 Ge1 116.634(12) 27 4_556
Ge1 Ba2 Ge1 91.826(2) 39_656 4_556
Ge1 Ba2 Ge1 59.201(17) 26_556 4_556
Ge1 Ba2 Ge1 159.434(11) . 4_556
Ge1 Ba2 Ge1 150.755(15) 14 4_556
Ge1 Ba2 Ge1 36.021(19) 16_545 4_556
Ge4 Ba2 Ge4 131.49(13) 41_666 46_656
Ge4 Ba2 Ge4 55.4(8) 2 46_656
Ge4 Ba2 Ge4 131.49(13) 42_666 46_656
Ge4 Ba2 Ge4 103.0(2) . 46_656
Ge4 Ba2 Ge4 71.4(9) 18_545 46_656
Ge4 Ba2 Ge4 55.4(8) 25_556 46_656
Ge4 Ba2 Ge4 71.4(9) 17_545 46_656
Ge4 Ba2 Ge4 103.0(2) 26_556 46_656
Ge3 Ba2 Ge4 136.3(2) 41_666 46_656
Ge3 Ba2 Ge4 59.7(6) 2 46_656
Ge3 Ba2 Ge4 99.7(2) . 46_656
Ge3 Ba2 Ge4 136.3(2) 42_666 46_656
Ge3 Ba2 Ge4 67.2(6) 18_545 46_656
Ge3 Ba2 Ge4 59.7(6) 25_556 46_656
Ge3 Ba2 Ge4 67.2(6) 17_545 46_656
Ge3 Ba2 Ge4 99.7(2) 26_556 46_656
Ge2 Ba2 Ge4 99.2(3) 33_656 46_656
Ge2 Ba2 Ge4 32.0(5) 29_556 46_656
Rh1 Ba2 Ge4 99.2(3) 33_656 46_656
Rh1 Ba2 Ge4 32.0(5) 29_556 46_656
Ge2 Ba2 Ge4 99.2(3) 9 46_656
Rh1 Ba2 Ge4 99.2(3) 9 46_656
Ge2 Ba2 Ge4 122.0(5) 5 46_656
Rh1 Ba2 Ge4 122.0(5) 5 46_656
Ge1 Ba2 Ge4 150.38(2) 37_666 46_656
Ge1 Ba2 Ge4 58.57(4) 27 46_656
Ge1 Ba2 Ge4 37.9(3) 39_656 46_656
Ge1 Ba2 Ge4 116.18(16) 26_556 46_656
Ge1 Ba2 Ge4 116.18(16) . 46_656
Ge1 Ba2 Ge4 150.379(19) 14 46_656
Ge1 Ba2 Ge4 37.9(3) 16_545 46_656
Ge1 Ba2 Ge4 58.57(4) 4_556 46_656
Ge4 Ba2 Ge4 55.4(8) 41_666 6_556
Ge4 Ba2 Ge4 131.49(12) 2 6_556
Ge4 Ba2 Ge4 103.0(2) 42_666 6_556
Ge4 Ba2 Ge4 131.49(13) . 6_556
Ge4 Ba2 Ge4 55.4(8) 18_545 6_556
Ge4 Ba2 Ge4 71.4(9) 25_556 6_556
Ge4 Ba2 Ge4 103.0(2) 17_545 6_556
Ge4 Ba2 Ge4 71.4(9) 26_556 6_556
Ge3 Ba2 Ge4 59.7(6) 41_666 6_556
Ge3 Ba2 Ge4 136.3(2) 2 6_556
Ge3 Ba2 Ge4 136.3(2) . 6_556
Ge3 Ba2 Ge4 99.7(2) 42_666 6_556
Ge3 Ba2 Ge4 59.7(6) 18_545 6_556
Ge3 Ba2 Ge4 67.2(6) 25_556 6_556
Ge3 Ba2 Ge4 99.7(2) 17_545 6_556
Ge3 Ba2 Ge4 67.2(6) 26_556 6_556
Ge2 Ba2 Ge4 32.0(5) 33_656 6_556
Ge2 Ba2 Ge4 99.2(3) 29_556 6_556
Rh1 Ba2 Ge4 32.0(5) 33_656 6_556
Rh1 Ba2 Ge4 99.2(3) 29_556 6_556
Ge2 Ba2 Ge4 122.0(5) 9 6_556
Rh1 Ba2 Ge4 122.0(5) 9 6_556
Ge2 Ba2 Ge4 99.2(3) 5 6_556
Rh1 Ba2 Ge4 99.2(3) 5 6_556
Ge1 Ba2 Ge4 58.57(4) 37_666 6_556
Ge1 Ba2 Ge4 150.38(2) 27 6_556
Ge1 Ba2 Ge4 116.18(15) 39_656 6_556
Ge1 Ba2 Ge4 37.9(3) 26_556 6_556
Ge1 Ba2 Ge4 150.38(2) . 6_556
Ge1 Ba2 Ge4 116.18(16) 14 6_556
Ge1 Ba2 Ge4 58.57(4) 16_545 6_556
Ge1 Ba2 Ge4 37.9(3) 4_556 6_556
Ge4 Ba2 Ge4 92.9(2) 46_656 6_556
Ge4 Ba2 Ge4 71.4(9) 41_666 45_666
Ge4 Ba2 Ge4 103.0(2) 2 45_666
Ge4 Ba2 Ge4 71.4(9) 42_666 45_666
Ge4 Ba2 Ge4 55.4(8) . 45_666
Ge4 Ba2 Ge4 131.49(12) 18_545 45_666
Ge4 Ba2 Ge4 103.0(2) 25_556 45_666
Ge4 Ba2 Ge4 131.49(12) 17_545 45_666
Ge4 Ba2 Ge4 55.4(8) 26_556 45_666
Ge3 Ba2 Ge4 67.2(6) 41_666 45_666
Ge3 Ba2 Ge4 99.7(2) 2 45_666
Ge3 Ba2 Ge4 59.7(6) . 45_666
Ge3 Ba2 Ge4 67.2(6) 42_666 45_666
Ge3 Ba2 Ge4 136.3(2) 18_545 45_666
Ge3 Ba2 Ge4 99.7(2) 25_556 45_666
Ge3 Ba2 Ge4 136.3(2) 17_545 45_666
Ge3 Ba2 Ge4 59.7(6) 26_556 45_666
Ge2 Ba2 Ge4 99.2(3) 33_656 45_666
Ge2 Ba2 Ge4 122.0(5) 29_556 45_666
Rh1 Ba2 Ge4 99.2(3) 33_656 45_666
Rh1 Ba2 Ge4 122.0(5) 29_556 45_666
Ge2 Ba2 Ge4 99.2(3) 9 45_666
Rh1 Ba2 Ge4 99.2(3) 9 45_666
Ge2 Ba2 Ge4 32.0(5) 5 45_666
Rh1 Ba2 Ge4 32.0(5) 5 45_666
Ge1 Ba2 Ge4 37.9(3) 37_666 45_666
Ge1 Ba2 Ge4 116.18(15) 27 45_666
Ge1 Ba2 Ge4 150.379(19) 39_656 45_666
Ge1 Ba2 Ge4 58.57(4) 26_556 45_666
Ge1 Ba2 Ge4 58.57(4) . 45_666
Ge1 Ba2 Ge4 37.9(3) 14 45_666
Ge1 Ba2 Ge4 150.38(2) 16_545 45_666
Ge1 Ba2 Ge4 116.18(15) 4_556 45_666
Ge4 Ba2 Ge4 154.0(10) 46_656 45_666
Ge4 Ba2 Ge4 92.9(2) 6_556 45_666
Ge4 Ba2 Ge4 103.0(2) 41_666 5
Ge4 Ba2 Ge4 71.4(9) 2 5
Ge4 Ba2 Ge4 55.4(8) 42_666 5
Ge4 Ba2 Ge4 71.4(9) . 5
Ge4 Ba2 Ge4 103.0(2) 18_545 5
Ge4 Ba2 Ge4 131.49(12) 25_556 5
Ge4 Ba2 Ge4 55.4(8) 17_545 5
Ge4 Ba2 Ge4 131.49(13) 26_556 5
Ge3 Ba2 Ge4 99.7(2) 41_666 5
Ge3 Ba2 Ge4 67.2(6) 2 5
Ge3 Ba2 Ge4 67.2(6) . 5
Ge3 Ba2 Ge4 59.7(6) 42_666 5
Ge3 Ba2 Ge4 99.7(2) 18_545 5
Ge3 Ba2 Ge4 136.3(2) 25_556 5
Ge3 Ba2 Ge4 59.7(6) 17_545 5
Ge3 Ba2 Ge4 136.3(2) 26_556 5
Ge2 Ba2 Ge4 122.0(5) 33_656 5
Ge2 Ba2 Ge4 99.2(3) 29_556 5
Rh1 Ba2 Ge4 122.0(5) 33_656 5
Rh1 Ba2 Ge4 99.2(3) 29_556 5
Ge2 Ba2 Ge4 32.0(5) 9 5
Rh1 Ba2 Ge4 32.0(5) 9 5
Ge2 Ba2 Ge4 99.2(3) 5 5
Rh1 Ba2 Ge4 99.2(3) 5 5
Ge1 Ba2 Ge4 116.18(16) 37_666 5
Ge1 Ba2 Ge4 37.9(3) 27 5
Ge1 Ba2 Ge4 58.57(4) 39_656 5
Ge1 Ba2 Ge4 150.38(2) 26_556 5
Ge1 Ba2 Ge4 37.9(3) . 5
Ge1 Ba2 Ge4 58.57(4) 14 5
Ge1 Ba2 Ge4 116.18(15) 16_545 5
Ge1 Ba2 Ge4 150.38(2) 4_556 5
Ge4 Ba2 Ge4 92.9(2) 46_656 5
Ge4 Ba2 Ge4 154.0(10) 6_556 5
Ge4 Ba2 Ge4 92.9(2) 45_666 5
Ge4 Ba2 Ge3 127.9(4) 41_666 46_656
Ge4 Ba2 Ge3 58.8(6) 2 46_656
Ge4 Ba2 Ge3 127.9(4) 42_666 46_656
Ge4 Ba2 Ge3 106.6(2) . 46_656
Ge4 Ba2 Ge3 67.5(6) 18_545 46_656
Ge4 Ba2 Ge3 58.8(6) 25_556 46_656
Ge4 Ba2 Ge3 67.5(6) 17_545 46_656
Ge4 Ba2 Ge3 106.6(2) 26_556 46_656
Ge3 Ba2 Ge3 132.56(5) 41_666 46_656
Ge3 Ba2 Ge3 63.0(4) 2 46_656
Ge3 Ba2 Ge3 103.15(12) . 46_656
Ge3 Ba2 Ge3 132.56(5) 42_666 46_656
Ge3 Ba2 Ge3 63.3(4) 18_545 46_656
Ge3 Ba2 Ge3 63.0(4) 25_556 46_656
Ge3 Ba2 Ge3 63.3(4) 17_545 46_656
Ge3 Ba2 Ge3 103.15(12) 26_556 46_656
Ge2 Ba2 Ge3 96.18(14) 33_656 46_656
Ge2 Ba2 Ge3 36.2(2) 29_556 46_656
Rh1 Ba2 Ge3 96.18(14) 33_656 46_656
Rh1 Ba2 Ge3 36.2(2) 29_556 46_656
Ge2 Ba2 Ge3 96.18(14) 9 46_656
Rh1 Ba2 Ge3 96.18(14) 9 46_656
Ge2 Ba2 Ge3 126.2(2) 5 46_656
Rh1 Ba2 Ge3 126.2(2) 5 46_656
Ge1 Ba2 Ge3 150.25(2) 37_666 46_656
Ge1 Ba2 Ge3 58.98(2) 27 46_656
Ge1 Ba2 Ge3 35.52(10) 39_656 46_656
Ge1 Ba2 Ge3 117.45(6) 26_556 46_656
Ge1 Ba2 Ge3 117.45(6) . 46_656
Ge1 Ba2 Ge3 150.25(2) 14 46_656
Ge1 Ba2 Ge3 35.52(10) 16_545 46_656
Ge1 Ba2 Ge3 58.98(2) 4_556 46_656
Ge4 Ba2 Ge3 4.2(3) 46_656 46_656
Ge4 Ba2 Ge3 91.96(11) 6_556 46_656
Ge4 Ba2 Ge3 158.2(7) 45_666 46_656
Ge4 Ba2 Ge3 91.96(11) 5 46_656
Ge4 Ba2 Ge3 58.8(6) 41_666 6_556
Ge4 Ba2 Ge3 127.9(4) 2 6_556
Ge4 Ba2 Ge3 106.6(2) 42_666 6_556
Ge4 Ba2 Ge3 127.9(4) . 6_556
Ge4 Ba2 Ge3 58.8(6) 18_545 6_556
Ge4 Ba2 Ge3 67.5(6) 25_556 6_556
Ge4 Ba2 Ge3 106.6(2) 17_545 6_556
Ge4 Ba2 Ge3 67.5(6) 26_556 6_556
Ge3 Ba2 Ge3 63.0(4) 41_666 6_556
Ge3 Ba2 Ge3 132.56(5) 2 6_556
Ge3 Ba2 Ge3 132.56(5) . 6_556
Ge3 Ba2 Ge3 103.15(12) 42_666 6_556
Ge3 Ba2 Ge3 63.0(4) 18_545 6_556
Ge3 Ba2 Ge3 63.3(4) 25_556 6_556
Ge3 Ba2 Ge3 103.15(12) 17_545 6_556
Ge3 Ba2 Ge3 63.3(4) 26_556 6_556
Ge2 Ba2 Ge3 36.2(2) 33_656 6_556
Ge2 Ba2 Ge3 96.18(14) 29_556 6_556
Rh1 Ba2 Ge3 36.2(2) 33_656 6_556
Rh1 Ba2 Ge3 96.18(14) 29_556 6_556
Ge2 Ba2 Ge3 126.2(2) 9 6_556
Rh1 Ba2 Ge3 126.2(2) 9 6_556
Ge2 Ba2 Ge3 96.18(14) 5 6_556
Rh1 Ba2 Ge3 96.18(14) 5 6_556
Ge1 Ba2 Ge3 58.98(2) 37_666 6_556
Ge1 Ba2 Ge3 150.25(2) 27 6_556
Ge1 Ba2 Ge3 117.45(6) 39_656 6_556
Ge1 Ba2 Ge3 35.52(10) 26_556 6_556
Ge1 Ba2 Ge3 150.25(2) . 6_556
Ge1 Ba2 Ge3 117.45(6) 14 6_556
Ge1 Ba2 Ge3 58.98(2) 16_545 6_556
Ge1 Ba2 Ge3 35.52(10) 4_556 6_556
Ge4 Ba2 Ge3 91.96(11) 46_656 6_556
Ge4 Ba2 Ge3 4.2(3) 6_556 6_556
Ge4 Ba2 Ge3 91.96(11) 45_666 6_556
Ge4 Ba2 Ge3 158.2(7) 5 6_556
Ge3 Ba2 Ge3 91.33(6) 46_656 6_556
Ge4 Ba2 Ge3 67.5(6) 41_666 45_666
Ge4 Ba2 Ge3 106.6(2) 2 45_666
Ge4 Ba2 Ge3 67.5(6) 42_666 45_666
Ge4 Ba2 Ge3 58.8(6) . 45_666
Ge4 Ba2 Ge3 127.9(4) 18_545 45_666
Ge4 Ba2 Ge3 106.6(2) 25_556 45_666
Ge4 Ba2 Ge3 127.9(4) 17_545 45_666
Ge4 Ba2 Ge3 58.8(6) 26_556 45_666
Ge3 Ba2 Ge3 63.3(4) 41_666 45_666
Ge3 Ba2 Ge3 103.15(12) 2 45_666
Ge3 Ba2 Ge3 63.0(4) . 45_666
Ge3 Ba2 Ge3 63.3(4) 42_666 45_666
Ge3 Ba2 Ge3 132.56(5) 18_545 45_666
Ge3 Ba2 Ge3 103.15(12) 25_556 45_666
Ge3 Ba2 Ge3 132.56(5) 17_545 45_666
Ge3 Ba2 Ge3 63.0(4) 26_556 45_666
Ge2 Ba2 Ge3 96.18(14) 33_656 45_666
Ge2 Ba2 Ge3 126.2(2) 29_556 45_666
Rh1 Ba2 Ge3 96.18(14) 33_656 45_666
Rh1 Ba2 Ge3 126.2(2) 29_556 45_666
Ge2 Ba2 Ge3 96.18(14) 9 45_666
Rh1 Ba2 Ge3 96.18(14) 9 45_666
Ge2 Ba2 Ge3 36.2(2) 5 45_666
Rh1 Ba2 Ge3 36.2(2) 5 45_666
Ge1 Ba2 Ge3 35.52(10) 37_666 45_666
Ge1 Ba2 Ge3 117.45(6) 27 45_666
Ge1 Ba2 Ge3 150.25(2) 39_656 45_666
Ge1 Ba2 Ge3 58.98(2) 26_556 45_666
Ge1 Ba2 Ge3 58.98(2) . 45_666
Ge1 Ba2 Ge3 35.52(10) 14 45_666
Ge1 Ba2 Ge3 150.25(2) 16_545 45_666
Ge1 Ba2 Ge3 117.45(6) 4_556 45_666
Ge4 Ba2 Ge3 158.2(7) 46_656 45_666
Ge4 Ba2 Ge3 91.96(11) 6_556 45_666
Ge4 Ba2 Ge3 4.2(3) 45_666 45_666
Ge4 Ba2 Ge3 91.96(11) 5 45_666
Ge3 Ba2 Ge3 162.5(4) 46_656 45_666
Ge3 Ba2 Ge3 91.33(6) 6_556 45_666
Ge4 Ba2 Ge3 106.6(2) 41_666 5
Ge4 Ba2 Ge3 67.5(6) 2 5
Ge4 Ba2 Ge3 58.8(6) 42_666 5
Ge4 Ba2 Ge3 67.5(6) . 5
Ge4 Ba2 Ge3 106.6(2) 18_545 5
Ge4 Ba2 Ge3 127.9(4) 25_556 5
Ge4 Ba2 Ge3 58.8(6) 17_545 5
Ge4 Ba2 Ge3 127.9(4) 26_556 5
Ge3 Ba2 Ge3 103.15(12) 41_666 5
Ge3 Ba2 Ge3 63.3(4) 2 5
Ge3 Ba2 Ge3 63.3(4) . 5
Ge3 Ba2 Ge3 63.0(4) 42_666 5
Ge3 Ba2 Ge3 103.15(12) 18_545 5
Ge3 Ba2 Ge3 132.56(5) 25_556 5
Ge3 Ba2 Ge3 63.0(4) 17_545 5
Ge3 Ba2 Ge3 132.56(5) 26_556 5
Ge2 Ba2 Ge3 126.2(2) 33_656 5
Ge2 Ba2 Ge3 96.18(14) 29_556 5
Rh1 Ba2 Ge3 126.2(2) 33_656 5
Rh1 Ba2 Ge3 96.18(14) 29_556 5
Ge2 Ba2 Ge3 36.2(2) 9 5
Rh1 Ba2 Ge3 36.2(2) 9 5
Ge2 Ba2 Ge3 96.18(14) 5 5
Rh1 Ba2 Ge3 96.18(14) 5 5
Ge1 Ba2 Ge3 117.45(6) 37_666 5
Ge1 Ba2 Ge3 35.52(10) 27 5
Ge1 Ba2 Ge3 58.98(2) 39_656 5
Ge1 Ba2 Ge3 150.25(2) 26_556 5
Ge1 Ba2 Ge3 35.52(10) . 5
Ge1 Ba2 Ge3 58.98(2) 14 5
Ge1 Ba2 Ge3 117.45(6) 16_545 5
Ge1 Ba2 Ge3 150.25(2) 4_556 5
Ge4 Ba2 Ge3 91.96(11) 46_656 5
Ge4 Ba2 Ge3 158.2(7) 6_556 5
Ge4 Ba2 Ge3 91.96(11) 45_666 5
Ge4 Ba2 Ge3 4.2(3) 5 5
Ge3 Ba2 Ge3 91.33(6) 46_656 5
Ge3 Ba2 Ge3 162.5(4) 6_556 5
Ge3 Ba2 Ge3 91.33(6) 45_666 5
Ge4 Rh1 Ge4 109.4(4) 14 9
Ge4 Rh1 Ge4 109.6(8) 14 37_665
Ge4 Rh1 Ge4 109.4(4) 9 37_665
Ge4 Rh1 Ge4 109.4(4) 14 34_565
Ge4 Rh1 Ge4 109.6(8) 9 34_565
Ge4 Rh1 Ge4 109.4(4) 37_665 34_565
Ge4 Rh1 Ge3 0.0(6) 14 14
Ge4 Rh1 Ge3 109.37(11) 9 14
Ge4 Rh1 Ge3 109.7(2) 37_665 14
Ge4 Rh1 Ge3 109.37(11) 34_565 14
Ge4 Rh1 Ge3 109.37(11) 14 9
Ge4 Rh1 Ge3 0.0(6) 9 9
Ge4 Rh1 Ge3 109.37(11) 37_665 9
Ge4 Rh1 Ge3 109.7(2) 34_565 9
Ge3 Rh1 Ge3 109.36(17) 14 9
Ge4 Rh1 Ge3 109.37(11) 14 34_565
Ge4 Rh1 Ge3 109.7(2) 9 34_565
Ge4 Rh1 Ge3 109.37(11) 37_665 34_565
Ge4 Rh1 Ge3 0.0(6) 34_565 34_565
Ge3 Rh1 Ge3 109.36(17) 14 34_565
Ge3 Rh1 Ge3 109.7(3) 9 34_565
Ge4 Rh1 Ge3 109.7(2) 14 37_665
Ge4 Rh1 Ge3 109.37(11) 9 37_665
Ge4 Rh1 Ge3 0.0(6) 37_665 37_665
Ge4 Rh1 Ge3 109.37(11) 34_565 37_665
Ge3 Rh1 Ge3 109.7(3) 14 37_665
Ge3 Rh1 Ge3 109.36(17) 9 37_665
Ge3 Rh1 Ge3 109.36(17) 34_565 37_665
Ge4 Rh1 Ba2 170.2(4) 14 33_565
Ge4 Rh1 Ba2 66.0(2) 9 33_565
Ge4 Rh1 Ba2 80.2(4) 37_665 33_565
Ge4 Rh1 Ba2 66.0(2) 34_565 33_565
Ge3 Rh1 Ba2 170.15(17) 14 33_565
Ge3 Rh1 Ba2 65.98(11) 9 33_565
Ge3 Rh1 Ba2 65.98(11) 34_565 33_565
Ge3 Rh1 Ba2 80.15(17) 37_665 33_565
Ge4 Rh1 Ba2 66.0(2) 14 29_665
Ge4 Rh1 Ba2 170.2(4) 9 29_665
Ge4 Rh1 Ba2 66.0(2) 37_665 29_665
Ge4 Rh1 Ba2 80.2(4) 34_565 29_665
Ge3 Rh1 Ba2 65.98(11) 14 29_665
Ge3 Rh1 Ba2 170.15(17) 9 29_665
Ge3 Rh1 Ba2 80.15(17) 34_565 29_665
Ge3 Rh1 Ba2 65.98(11) 37_665 29_665
Ba2 Rh1 Ba2 120.0 33_565 29_665
Ge4 Rh1 Ba2 66.0(2) 14 5
Ge4 Rh1 Ba2 80.2(4) 9 5
Ge4 Rh1 Ba2 66.0(2) 37_665 5
Ge4 Rh1 Ba2 170.2(4) 34_565 5
Ge3 Rh1 Ba2 65.98(11) 14 5
Ge3 Rh1 Ba2 80.15(17) 9 5
Ge3 Rh1 Ba2 170.15(17) 34_565 5
Ge3 Rh1 Ba2 65.98(11) 37_665 5
Ba2 Rh1 Ba2 120.0 33_565 5
Ba2 Rh1 Ba2 90.0 29_665 5
Ge4 Rh1 Ba2 80.2(4) 14 9
Ge4 Rh1 Ba2 66.0(2) 9 9
Ge4 Rh1 Ba2 170.2(4) 37_665 9
Ge4 Rh1 Ba2 66.0(2) 34_565 9
Ge3 Rh1 Ba2 80.15(17) 14 9
Ge3 Rh1 Ba2 65.98(11) 9 9
Ge3 Rh1 Ba2 65.98(11) 34_565 9
Ge3 Rh1 Ba2 170.15(17) 37_665 9
Ba2 Rh1 Ba2 90.0 33_565 9
Ba2 Rh1 Ba2 120.0 29_665 9
Ba2 Rh1 Ba2 120.0 5 9
Ge4 Ge2 Ge4 109.4(4) 14 9
Ge4 Ge2 Ge4 109.6(8) 14 37_665
Ge4 Ge2 Ge4 109.4(4) 9 37_665
Ge4 Ge2 Ge4 109.4(4) 14 34_565
Ge4 Ge2 Ge4 109.6(8) 9 34_565
Ge4 Ge2 Ge4 109.4(4) 37_665 34_565
Ge4 Ge2 Ge3 0.0(6) 14 14
Ge4 Ge2 Ge3 109.37(11) 9 14
Ge4 Ge2 Ge3 109.7(2) 37_665 14
Ge4 Ge2 Ge3 109.37(11) 34_565 14
Ge4 Ge2 Ge3 109.37(11) 14 9
Ge4 Ge2 Ge3 0.0(6) 9 9
Ge4 Ge2 Ge3 109.37(11) 37_665 9
Ge4 Ge2 Ge3 109.7(2) 34_565 9
Ge3 Ge2 Ge3 109.36(17) 14 9
Ge4 Ge2 Ge3 109.37(11) 14 34_565
Ge4 Ge2 Ge3 109.7(2) 9 34_565
Ge4 Ge2 Ge3 109.37(11) 37_665 34_565
Ge4 Ge2 Ge3 0.0(6) 34_565 34_565
Ge3 Ge2 Ge3 109.36(17) 14 34_565
Ge3 Ge2 Ge3 109.7(3) 9 34_565
Ge4 Ge2 Ge3 109.7(2) 14 37_665
Ge4 Ge2 Ge3 109.37(11) 9 37_665
Ge4 Ge2 Ge3 0.0(6) 37_665 37_665
Ge4 Ge2 Ge3 109.37(11) 34_565 37_665
Ge3 Ge2 Ge3 109.7(3) 14 37_665
Ge3 Ge2 Ge3 109.36(17) 9 37_665
Ge3 Ge2 Ge3 109.36(17) 34_565 37_665
Ge4 Ge2 Ba2 170.2(4) 14 33_565
Ge4 Ge2 Ba2 66.0(2) 9 33_565
Ge4 Ge2 Ba2 80.2(4) 37_665 33_565
Ge4 Ge2 Ba2 66.0(2) 34_565 33_565
Ge3 Ge2 Ba2 170.15(17) 14 33_565
Ge3 Ge2 Ba2 65.98(11) 9 33_565
Ge3 Ge2 Ba2 65.98(11) 34_565 33_565
Ge3 Ge2 Ba2 80.15(17) 37_665 33_565
Ge4 Ge2 Ba2 66.0(2) 14 29_665
Ge4 Ge2 Ba2 170.2(4) 9 29_665
Ge4 Ge2 Ba2 66.0(2) 37_665 29_665
Ge4 Ge2 Ba2 80.2(4) 34_565 29_665
Ge3 Ge2 Ba2 65.98(11) 14 29_665
Ge3 Ge2 Ba2 170.15(17) 9 29_665
Ge3 Ge2 Ba2 80.15(17) 34_565 29_665
Ge3 Ge2 Ba2 65.98(11) 37_665 29_665
Ba2 Ge2 Ba2 120.0 33_565 29_665
Ge4 Ge2 Ba2 66.0(2) 14 5
Ge4 Ge2 Ba2 80.2(4) 9 5
Ge4 Ge2 Ba2 66.0(2) 37_665 5
Ge4 Ge2 Ba2 170.2(4) 34_565 5
Ge3 Ge2 Ba2 65.98(11) 14 5
Ge3 Ge2 Ba2 80.15(17) 9 5
Ge3 Ge2 Ba2 170.15(17) 34_565 5
Ge3 Ge2 Ba2 65.98(11) 37_665 5
Ba2 Ge2 Ba2 120.0 33_565 5
Ba2 Ge2 Ba2 90.0 29_665 5
Ge4 Ge2 Ba2 80.2(4) 14 9
Ge4 Ge2 Ba2 66.0(2) 9 9
Ge4 Ge2 Ba2 170.2(4) 37_665 9
Ge4 Ge2 Ba2 66.0(2) 34_565 9
Ge3 Ge2 Ba2 80.15(17) 14 9
Ge3 Ge2 Ba2 65.98(11) 9 9
Ge3 Ge2 Ba2 65.98(11) 34_565 9
Ge3 Ge2 Ba2 170.15(17) 37_665 9
Ba2 Ge2 Ba2 90.0 33_565 9
Ba2 Ge2 Ba2 120.0 29_665 9
Ba2 Ge2 Ba2 120.0 5 9
Ge1 Ge1 Ge3 108.2(4) 14 9
Ge1 Ge1 Ge3 108.2(4) 14 5
Ge3 Ge1 Ge3 110.7(3) 9 5
Ge1 Ge1 Ge3 108.2(4) 14 .
Ge3 Ge1 Ge3 110.7(3) 9 .
Ge3 Ge1 Ge3 110.7(3) 5 .
Ge1 Ge1 Ge4 101.4(7) 14 .
Ge3 Ge1 Ge4 112.4(6) 9 .
Ge3 Ge1 Ge4 115.2(5) 5 .
Ge3 Ge1 Ge4 7.1(4) . .
Ge1 Ge1 Ge4 101.4(7) 14 9
Ge3 Ge1 Ge4 7.1(4) 9 9
Ge3 Ge1 Ge4 112.4(6) 5 9
Ge3 Ge1 Ge4 115.2(5) . 9
Ge4 Ge1 Ge4 116.2(4) . 9
Ge1 Ge1 Ge4 101.4(7) 14 5
Ge3 Ge1 Ge4 115.2(5) 9 5
Ge3 Ge1 Ge4 7.1(4) 5 5
Ge3 Ge1 Ge4 112.4(6) . 5
Ge4 Ge1 Ge4 116.2(4) . 5
Ge4 Ge1 Ge4 116.2(4) 9 5
Ge1 Ge1 Ba1 180.00(5) 14 .
Ge3 Ge1 Ba1 71.8(4) 9 .
Ge3 Ge1 Ba1 71.8(4) 5 .
Ge3 Ge1 Ba1 71.8(4) . .
Ge4 Ge1 Ba1 78.6(7) . .
Ge4 Ge1 Ba1 78.6(7) 9 .
Ge4 Ge1 Ba1 78.6(7) 5 .
Ge1 Ge1 Ba2 71.990(9) 14 5
Ge3 Ge1 Ba2 76.3(3) 9 5
Ge3 Ge1 Ba2 62.43(15) 5 5
Ge3 Ge1 Ba2 172.13(18) . 5
Ge4 Ge1 Ba2 170.7(5) . 5
Ge4 Ge1 Ba2 72.0(4) 9 5
Ge4 Ge1 Ba2 60.3(3) 5 5
Ba1 Ge1 Ba2 108.010(9) . 5
Ge1 Ge1 Ba2 71.990(9) 14 .
Ge3 Ge1 Ba2 172.13(18) 9 .
Ge3 Ge1 Ba2 76.3(3) 5 .
Ge3 Ge1 Ba2 62.43(15) . .
Ge4 Ge1 Ba2 60.3(3) . .
Ge4 Ge1 Ba2 170.7(5) 9 .
Ge4 Ge1 Ba2 72.0(4) 5 .
Ba1 Ge1 Ba2 108.010(9) . .
Ba2 Ge1 Ba2 110.892(9) 5 .
Ge1 Ge1 Ba2 71.990(9) 14 9
Ge3 Ge1 Ba2 62.43(15) 9 9
Ge3 Ge1 Ba2 172.13(18) 5 9
Ge3 Ge1 Ba2 76.3(3) . 9
Ge4 Ge1 Ba2 72.0(4) . 9
Ge4 Ge1 Ba2 60.3(3) 9 9
Ge4 Ge1 Ba2 170.7(5) 5 9
Ba1 Ge1 Ba2 108.010(9) . 9
Ba2 Ge1 Ba2 110.892(9) 5 9
Ba2 Ge1 Ba2 110.892(9) . 9
Ge1 Ge1 Ba2 107.832(6) 14 33_565
Ge3 Ge1 Ba2 2.52(15) 9 33_565
Ge3 Ge1 Ba2 113.0(3) 5 33_565
Ge3 Ge1 Ba2 108.67(14) . 33_565
Ge4 Ge1 Ba2 110.2(3) . 33_565
Ge4 Ge1 Ba2 7.7(6) 9 33_565
Ge4 Ge1 Ba2 117.7(5) 5 33_565
Ba1 Ge1 Ba2 72.168(6) . 33_565
Ba2 Ge1 Ba2 78.366(1) 5 33_565
Ba2 Ge1 Ba2 169.6 . 33_565
Ba2 Ge1 Ba2 60.133(2) 9 33_565
Ge4 Ge3 Ge3 125(4) . 2
Ge4 Ge3 Ge1 106(2) . 28
Ge3 Ge3 Ge1 107.0(3) 2 28
Ge4 Ge3 Ge1 106(2) . .
Ge3 Ge3 Ge1 107.0(3) 2 .
Ge1 Ge3 Ge1 104.3(3) 28 .
Ge4 Ge3 Ge2 0(4) . 5
Ge3 Ge3 Ge2 125.15(17) 2 5
Ge1 Ge3 Ge2 105.8(4) 28 5
Ge1 Ge3 Ge2 105.8(4) . 5
Ge4 Ge3 Rh1 0(4) . 5
Ge3 Ge3 Rh1 125.15(17) 2 5
Ge1 Ge3 Rh1 105.8(4) 28 5
Ge1 Ge3 Rh1 105.8(4) . 5
Ge2 Ge3 Rh1 0.0 5 5
Ge4 Ge3 Ge4 119(4) . 2
Ge3 Ge3 Ge4 5.8(5) 2 2
Ge1 Ge3 Ge4 110.22(17) 28 2
Ge1 Ge3 Ge4 110.22(17) . 2
Ge2 Ge3 Ge4 119.3(6) 5 2
Rh1 Ge3 Ge4 119.3(6) 5 2
Ge4 Ge3 Ba1 166(4) . .
Ge3 Ge3 Ba1 69.49(15) 2 .
Ge1 Ge3 Ba1 66.2(3) 28 .
Ge1 Ge3 Ba1 66.2(3) . .
Ge2 Ge3 Ba1 165.4(3) 5 .
Rh1 Ge3 Ba1 165.4(3) 5 .
Ge4 Ge3 Ba1 75.3(3) 2 .
Ge4 Ge3 Ba2 74(2) . .
Ge3 Ge3 Ba2 69.8(2) 2 .
Ge1 Ge3 Ba2 175.7(3) 28 .
Ge1 Ge3 Ba2 79.59(5) . .
Ge2 Ge3 Ba2 74.5(2) 5 .
Rh1 Ge3 Ba2 74.5(2) 5 .
Ge4 Ge3 Ba2 66.4(4) 2 .
Ba1 Ge3 Ba2 114.4(3) . .
Ge4 Ge3 Ba2 74(2) . 25_556
Ge3 Ge3 Ba2 69.8(2) 2 25_556
Ge1 Ge3 Ba2 79.59(5) 28 25_556
Ge1 Ge3 Ba2 175.7(3) . 25_556
Ge2 Ge3 Ba2 74.5(2) 5 25_556
Rh1 Ge3 Ba2 74.5(2) 5 25_556
Ge4 Ge3 Ba2 66.4(4) 2 25_556
Ba1 Ge3 Ba2 114.4(3) . 25_556
Ba2 Ge3 Ba2 96.5(2) . 25_556
Ge4 Ge3 Ba2 64(4) . 9
Ge3 Ge3 Ba2 171.2(2) 2 9
Ge1 Ge3 Ba2 68.2(2) 28 9
Ge1 Ge3 Ba2 68.2(2) . 9
Ge2 Ge3 Ba2 63.6(3) 5 9
Rh1 Ge3 Ba2 63.6(3) 5 9
Ge4 Ge3 Ba2 177.1(4) 2 9
Ba1 Ge3 Ba2 101.75(18) . 9
Ba2 Ge3 Ba2 115.3(3) . 9
Ba2 Ge3 Ba2 115.3(3) 25_556 9
Ge3 Ge4 Ge2 180(4) . 5
Ge3 Ge4 Rh1 180(4) . 5
Ge2 Ge4 Rh1 0.0 5 5
Ge3 Ge4 Ge1 67(2) . 28
Ge2 Ge4 Ge1 112.9(7) 5 28
Rh1 Ge4 Ge1 112.9(7) 5 28
Ge3 Ge4 Ge1 67(2) . .
Ge2 Ge4 Ge1 112.9(7) 5 .
Rh1 Ge4 Ge1 112.9(7) 5 .
Ge1 Ge4 Ge1 98.2(9) 28 .
Ge3 Ge4 Ge3 49(3) . 2
Ge2 Ge4 Ge3 131.0(8) 5 2
Rh1 Ge4 Ge3 131.0(8) 5 2
Ge1 Ge4 Ge3 98.2(7) 28 2
Ge1 Ge4 Ge3 98.2(7) . 2
Ge3 Ge4 Ge4 55(4) . 2
Ge2 Ge4 Ge4 125.2(4) 5 2
Rh1 Ge4 Ge4 125.2(4) 5 2
Ge1 Ge4 Ge4 101.9(5) 28 2
Ge1 Ge4 Ge4 101.9(5) . 2
Ge3 Ge4 Ge4 5.8(5) 2 2
Ge3 Ge4 Ba2 100(2) . .
Ge2 Ge4 Ba2 79.8(6) 5 .
Rh1 Ge4 Ba2 79.8(6) 5 .
Ge1 Ge4 Ba2 166.7(12) 28 .
Ge1 Ge4 Ba2 79.71(8) . .
Ge3 Ge4 Ba2 69.3(4) 2 .
Ge4 Ge4 Ba2 66.0(4) 2 .
Ge3 Ge4 Ba2 100(2) . 25_556
Ge2 Ge4 Ba2 79.8(6) 5 25_556
Rh1 Ge4 Ba2 79.8(6) 5 25_556
Ge1 Ge4 Ba2 79.71(8) 28 25_556
Ge1 Ge4 Ba2 166.7(12) . 25_556
Ge3 Ge4 Ba2 69.3(4) 2 25_556
Ge4 Ge4 Ba2 66.0(4) 2 25_556
Ba2 Ge4 Ba2 99.3(5) . 25_556
Ge3 Ge4 Ba1 13(4) . .
Ge2 Ge4 Ba1 166.6(6) 5 .
Rh1 Ge4 Ba1 166.6(6) 5 .
Ge1 Ge4 Ba1 60.0(7) 28 .
Ge1 Ge4 Ba1 60.0(7) . .
Ge3 Ge4 Ba1 62.4(4) 2 .
Ge4 Ge4 Ba1 68.3(2) 2 .
Ba2 Ge4 Ba1 108.5(6) . .
Ba2 Ge4 Ba1 108.5(6) 25_556 .
Ge3 Ge4 Ba2 112(4) . 9
Ge2 Ge4 Ba2 67.8(5) 5 9
Rh1 Ge4 Ba2 67.8(5) 5 9
Ge1 Ge4 Ba2 70.1(3) 28 9
Ge1 Ge4 Ba2 70.1(3) . 9
Ge3 Ge4 Ba2 161.2(9) 2 9
Ge4 Ge4 Ba2 167.0(5) 2 9
Ba2 Ge4 Ba2 120.6(5) . 9
Ba2 Ge4 Ba2 120.6(5) 25_556 9
Ba1 Ge4 Ba2 98.7(5) . 9
Ge3 Ge4 Ba2 174(4) . 33_566
Ge2 Ge4 Ba2 6.2(2) 5 33_566
Rh1 Ge4 Ba2 6.2(2) 5 33_566
Ge1 Ge4 Ba2 109.2(7) 28 33_566
Ge1 Ge4 Ba2 109.2(7) . 33_566
Ge3 Ge4 Ba2 137.3(6) 2 33_566
Ge4 Ge4 Ba2 131.43(15) 2 33_566
Ba2 Ge4 Ba2 83.8(6) . 33_566
Ba2 Ge4 Ba2 83.8(6) 25_556 33_566
Ba1 Ge4 Ba2 160.3(3) . 33_566
Ba2 Ge4 Ba2 61.6(4) 9 33_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 Ge1 3.4059(9) 25
Ba1 Ge1 3.4059(9) .
Ba1 Ge1 3.4059(9) 28
Ba1 Ge1 3.4059(9) 4
Ba1 Ge1 3.4059(9) 27
Ba1 Ge1 3.4059(9) 3
Ba1 Ge1 3.4059(9) 26
Ba1 Ge1 3.4059(9) 2
Ba1 Ge3 3.535(15) 33
Ba1 Ge3 3.535(15) 9
Ba1 Ge3 3.535(15) 29
Ba1 Ge3 3.535(15) 5
Ba2 Ge4 3.513(12) 41_666
Ba2 Ge4 3.513(12) 2
Ba2 Ge4 3.513(12) 42_666
Ba2 Ge4 3.513(12) .
Ba2 Ge4 3.513(12) 18_545
Ba2 Ge4 3.513(12) 25_556
Ba2 Ge4 3.513(12) 17_545
Ba2 Ge4 3.513(12) 26_556
Ba2 Ge3 3.588(6) 41_666
Ba2 Ge3 3.588(6) 2
Ba2 Ge3 3.588(6) .
Ba2 Ge3 3.588(6) 42_666
Ba2 Ge3 3.588(6) 18_545
Ba2 Ge3 3.588(6) 25_556
Ba2 Ge3 3.588(6) 17_545
Ba2 Ge3 3.588(6) 26_556
Ba2 Ge2 3.7859(7) 33_656
Ba2 Ge2 3.7859(7) 29_556
Ba2 Rh1 3.7859(7) 33_656
Ba2 Rh1 3.7859(7) 29_556
Ba2 Ge2 3.7859(7) 9
Ba2 Rh1 3.7859(7) 9
Ba2 Ge2 3.7859(7) 5
Ba2 Rh1 3.7859(7) 5
Ba2 Ge1 3.9809(8) 37_666
Ba2 Ge1 3.9809(8) 27
Ba2 Ge1 3.9809(8) 39_656
Ba2 Ge1 3.9809(8) 26_556
Ba2 Ge1 3.9809(8) .
Ba2 Ge1 3.9809(8) 14
Ba2 Ge1 3.9809(8) 16_545
Ba2 Ge1 3.9809(8) 4_556
Ba2 Ge4 4.029(16) 46_656
Ba2 Ge4 4.029(16) 6_556
Ba2 Ge4 4.029(16) 45_666
Ba2 Ge4 4.029(16) 5
Ba2 Ge3 4.164(11) 46_656
Ba2 Ge3 4.164(11) 6_556
Ba2 Ge3 4.164(11) 45_666
Ba2 Ge3 4.164(11) 5
Rh1 Ge4 2.17(3) 14
Rh1 Ge4 2.17(3) 9
Rh1 Ge4 2.17(3) 37_665
Rh1 Ge4 2.17(3) 34_565
Rh1 Ge3 2.499(16) 14
Rh1 Ge3 2.499(16) 9
Rh1 Ge3 2.499(16) 34_565
Rh1 Ge3 2.499(16) 37_665
Rh1 Ba2 3.7859(7) 33_565
Rh1 Ba2 3.7859(7) 29_665
Rh1 Ba2 3.7859(7) 5
Rh1 Ba2 3.7859(7) 9
Ge2 Ge4 2.17(3) 14
Ge2 Ge4 2.17(3) 9
Ge2 Ge4 2.17(3) 37_665
Ge2 Ge4 2.17(3) 34_565
Ge2 Ge3 2.499(16) 14
Ge2 Ge3 2.499(16) 9
Ge2 Ge3 2.499(16) 34_565
Ge2 Ge3 2.499(16) 37_665
Ge2 Ba2 3.7859(7) 33_565
Ge2 Ba2 3.7859(7) 29_665
Ge2 Ba2 3.7859(7) 5
Ge2 Ba2 3.7859(7) 9
Ge1 Ge1 2.4617(15) 14
Ge1 Ge3 2.491(5) 9
Ge1 Ge3 2.491(5) 5
Ge1 Ge3 2.491(5) .
Ge1 Ge4 2.602(17) .
Ge1 Ge4 2.602(17) 9
Ge1 Ge4 2.602(17) 5
Ge1 Ba2 3.9809(8) 5
Ge1 Ba2 3.9809(8) 9
Ge1 Ba2 6.0749(11) 33_565
Ge3 Ge4 0.33(2) .
Ge3 Ge3 2.48(2) 2
Ge3 Ge1 2.491(5) 28
Ge3 Ge2 2.499(16) 5
Ge3 Rh1 2.499(16) 5
Ge3 Ge4 2.68(3) 2
Ge3 Ba2 3.588(6) 25_556
Ge3 Ba2 4.164(11) 9
Ge4 Ge2 2.17(3) 5
Ge4 Rh1 2.17(3) 5
Ge4 Ge1 2.602(17) 28
Ge4 Ge3 2.68(3) 2
Ge4 Ge4 2.86(4) 2
Ge4 Ba2 3.513(12) 25_556
Ge4 Ba2 4.029(16) 9
Ge4 Ba2 5.93(3) 33_566
